| ||Format||Pages||Price|| |
|3||$42.00||  ADD TO CART|
|Hardcopy (shipping and handling)||3||$42.00||  ADD TO CART|
Significance and Use
5.1 This method is intended to provide a generalized procedure for determining the stability of cellulosic pulp fibers exposed to alkaline environments. Specifically, this method allows various pulp types to be compared with respect to the effect of exposure to alkaline conditions on the strength of individual cellulosic fibers based on a zero-span tensile test. The time intervals listed in the procedure are not critical, and more intervals of shorter or longer duration may be added. In addition, the procedure may be simplified by removing some of the intermediate intervals so long as a range of intervals is determined. An example of a simplified procedure would be to determine 4 intervals (for example, 1 day, 1 week, 2 weeks, 4 weeks; or 1 day, 3 day, 7 day, 14 day).
5.2 The specified solution (1N NaOH) is strongly alkaline. Although this alkali concentration is higher than some environments that would be simulated by this test, the stronger pH provides better differentiation between different cellulose fiber types. Although alkaline stability based on other alkalis (for example, KOH, Ca(OH)2, etc.) at a different concentration could be determined by this method, 1N NaOH is to be considered the standard solution. Alkaline stability results from other treatments may be reported in addition to the standard solution if the additional solution(s) provide useful information.
1.1 This test method describes a procedure for determining the effect of exposure to alkaline environments on the strength of cellulose fibers. An alkaline environment is defined to be any matrix in which the pH is greater than 8 for a period of 2 or more hours.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
TAPPI (Technical Association of the Pulp & Paper Industry) StandardsT 231 Zero-span Breaking Strength of Pulp (Dry Zero-span Tensile)
D1348 Test Methods for Moisture in Cellulose
D1695 Terminology of Cellulose and Cellulose Derivatives
ICS Number Code 85.040 (Pulps)
UNSPSC Code 11151500(Fibers)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D6942-03(2012), Standard Test Method for Stability of Cellulose Fibers in Alkaline Environments, ASTM International, West Conshohocken, PA, 2012, www.astm.orgBack to Top